# ASTM A182 Grade F11 Class 2 (K11572) Steel

ASTM A182 grade F11 class 2 is an alloy steel formulated for primary forming into wrought products. Cited properties are appropriate for the annealed condition. Grade F11 Class 2 is the ASTM designation for this material. K11572 is the UNS number.

It has a moderately low thermal conductivity and a moderately low tensile strength among wrought alloy steels in the same category.

The graph bars on the material properties cards below compare ASTM A182 grade F11 class 2 to: wrought alloy steels in the same category (top), all iron alloys (middle), and the entire database (bottom). A full bar means this is the highest value in the relevant set. A half-full bar means it's 50% of the highest, and so on.

## Mechanical Properties

Brinell Hardness

180

Elastic (Young's, Tensile) Modulus

190 *GPa* 27 *x 10 ^{6} psi*

Elongation at Break

22 *%*

Fatigue Strength

220 *MPa* 32 *x 10 ^{3} psi*

Poisson's Ratio

0.29

Reduction in Area

34 *%*

Shear Modulus

73 *GPa* 11 *x 10 ^{6} psi*

Shear Strength

340 *MPa* 50 *x 10 ^{3} psi*

Tensile Strength: Ultimate (UTS)

540 *MPa* 79 *x 10 ^{3} psi*

Tensile Strength: Yield (Proof)

310 *MPa* 45 *x 10 ^{3} psi*

## Thermal Properties

Latent Heat of Fusion

260 *J/g*

Maximum Temperature: Mechanical

430 *°C* 810 *°F*

Melting Completion (Liquidus)

1460 *°C* 2660 *°F*

Melting Onset (Solidus)

1420 *°C* 2580 *°F*

Specific Heat Capacity

470 *J/kg-K* 0.11 *BTU/lb-°F*

Thermal Conductivity

39 *W/m-K* 23 *BTU/h-ft-°F*

Thermal Expansion

13 *µm/m-K*

## Electrical Properties

Electrical Conductivity: Equal Volume

7.4 *% IACS*

Electrical Conductivity: Equal Weight (Specific)

8.6 *% IACS*

## Otherwise Unclassified Properties

Base Metal Price

2.9 *% relative*

Density

7.8 *g/cm ^{3}* 490

*lb/ft*

^{3}Embodied Carbon

1.6 *kg CO _{2}/kg material*

Embodied Energy

21 *MJ/kg* 9.1 *x 10 ^{3} BTU/lb*

Embodied Water

53 *L/kg* 6.3 *gal/lb*

## Common Calculations

PREN (Pitting Resistance)

3.0

Resilience: Ultimate (Unit Rupture Work)

100 *MJ/m ^{3}*

Resilience: Unit (Modulus of Resilience)

260 *kJ/m ^{3}*

Stiffness to Weight: Axial

13 *points*

Stiffness to Weight: Bending

24 *points*

Strength to Weight: Axial

19 *points*

Strength to Weight: Bending

19 *points*

Thermal Diffusivity

11 *mm ^{2}/s*

Thermal Shock Resistance

16 *points*

## Alloy Composition

Among alloy steels, the composition of ASTM A182 grade F11 class 2 is notable for containing a comparatively high amount of chromium (Cr). Chromium is used to improve corrosion resistance and most mechanical properties (particularly at higher temperatures).

Fe | 95.8 to 97.7 | |

Cr | 1.0 to 1.5 | |

Si | 0.5 to 1.0 | |

Mn | 0.3 to 0.8 | |

Mo | 0.44 to 0.65 | |

C | 0.1 to 0.2 | |

P | 0 to 0.040 | |

S | 0 to 0.040 |

All values are % weight. Ranges represent what is permitted under applicable standards.

## Followup Questions

## Similar Alloys

## Further Reading

ASTM A182: Standard Specification for Forged or Rolled Alloy and Stainless Steel Pipe Flanges, Forged Fittings, and Valves and Parts for High-Temperature Service